- Nano Express
- Open Access
Synthesis and Characterization of Cobalt-Doped WS2 Nanorods for Lithium Battery Applications
© The Author(s) 2010
- Received: 16 March 2010
- Accepted: 7 May 2010
- Published: 23 May 2010
Cobalt-doped tungsten disulfide nanorods were synthesized by an approach involving exfoliation, intercalation, and the hydrothermal process, using commercial WS2 powder as the precursor and n-butyllithium as the exfoliating reagent. XRD results indicate that the crystal phase of the sample is 2H-WS2. TEM images show that the sample consists of bamboo-like nanorods with a diameter of around 20 nm and a length of about 200 nm. The Co-doped WS2 nanorods exhibit the reversible capacity of 568 mAh g−1 in a voltage range of 0.01–3.0 V versus Li/Li+. As an electrode material for the lithium battery, the Co-doped WS2 nanorods show enhanced charge capacity and cycling stability compared with the raw WS2 powder.
- Tungsten disulfide
- Chemical synthesis
- Electrochemical properties
- Electrode materials
- Hydrothermal method
Due to its distinctive layer structure and electronic properties, the inorganic fullerene-like structure of MS2(M = Mo, W) has been attracting considerable attention and has been investigated extensively for various applications. The properties of the metal disulfide nanomaterials with novel morphology are better than those of their bulk forms. WS2 and MoS2 nanomaterials have shown excellent properties and have potential applications in various fields, such as scanning probe microscopy , solid-state lubricants , heterogeneous catalysis , and electrochemical hydrogen storage . In order to investigate their properties and applications in these fields systematically, several methods have been reported to prepare nanoscale MS2, such as gas–solid or gas phase reaction , pulsed laser deposition , a self-transformation process , and sulfidation of the MoO3 nanofibers under a H2S/H2 steam at 350–600°C . However, almost all the methods are based on utilizing high temperature reactions or dangerous gases, such as H2 and H2S. On the other hand, the formation of nanosized MoS2 or WS2 polyhedral or onion crystals is, similar to the case of carbon onion crystals, a rare event . From this point of view, it is interesting and valuable to find a new large-scale approach to synthesize metal disulfide nanoparticles.
Since the 1970s, lamellar disulfide has been intensively studied, especially via the intercalation technique [10–12]. During intercalation, the coordination patterns of lamellar disulfide change greatly, and numerous defects are introduced, which enable doping of other ions [13, 14]. On the other hand, after transition metal cations have entered the WS2 or MoS2 matrix, there are changes in the bonding properties of the matrix and the S–M–S bond angles [14–16]. Golub et al.  described room temperature preparation of new ternary metal sulfides M x MoS2 (M = Cu, Ag) by exfoliation–restacking technique. First, the MoS2 powder is exfoliated into lamellae or monolayers by n-butyllithium to form Li x MoS2. Then (MoS2) x− is formed by the reaction of Li x WS2 with water. They supposed that ternary metal sulfides M x MoS2 could be obtained using (MoS2) x− single layers dispersed in aqueous media and salts of metals which could favor the formation of M–S rather than M–O(OH, H2O) bonds. Thus, the (MoS2) x− single layers in the dispersions have henceforth to be considered not only as macroanions but also as reducing agents. For the MoS2, the negative charge of (MoS2) x− and consequently the cluster structure of S–Mo–S layers with Mo–Mo metal bonding can be effectively stabilized in restacked compounds by introduction into the structure of counterions covalently bonded to the matrix. So it is possible the same reason for the WS2, the introduction of cobalt ion into the matrix of WS2 can stabilize the WS2. Li et al. [17, 18] utilized these bond changes and fabricated transition metal-doped disulfide nanotubes successfully by exfoliation–intercalation through hydrothermal adulteration, using lamellar metal disulfide as the precursors.
WS2 and MoS2 could be electrode materials for rechargeable batteries due to the existence of van der Waals forces across the gaps between the S–M–S sheets, which can provide the space for guest reactants in intercalation reactions . A few attempts have been made to investigate the electrochemical activity of MS2 (M = Mo, W, etc.) electrodes. For example, Feng  reported that WS2 nanoflakes prepared by a rheological phase reaction had better lithium intercalation/deintercalation behavior than other forms of WS2. Wang  prepared WS2 nanotubes and reported that the WS2 nanotube electrode delivered a lithium insertion capacity of 915 mAh g−1, which is much higher than for WS2 powder.
As other approach to explore new electrode materials for Li-battery, nanosized transition metal oxides have been attracting much attention in recent years. Poizot et al.  reported the high performance as anode materials in lithium ion batteries for nanosized transition metal oxides such as nickel oxide, cobalt oxide, and iron oxide. Among them, cobalt oxide demonstrated the best electrochemical properties. In this regard, Co-containing species can be promising intercalants to modify the lamellar disulfides. In this paper, bamboo-like Co-doped WS2 nanorods were synthesized on a large scale by an approach involving exfoliation–intercalation–hydrothermal treatment, using lamellar tungsten disulfide as the precursor, and the morphology, chemical components, and Raman spectrum are reported. The cobalt-doped WS2 nanorods can reversibly store lithium with a capacity of 568 mAh g−1 over a voltage range of 0.01–3.0 V versus Li/Li+ and show good cycling stability. To the best of our knowledge, this is the first time that transition metal-doped WS2 nanorods have been synthesized and their applications in lithium ion batteries systematically investigated.
Under N2 atmosphere at room temperature for a week, 8.2 g of WS2 powder was exfoliated by 2.9 M of n-butyllithium (15 ml) in a container, rinsed in hexane six times, and vacuum dried at 80°C overnight. Then, 0.6 g of Li x WS2 was put into a 50 ml autoclave with a Teflon-lined inner wall, and 30 ml of 0.2 M CoCl2 aqueous solution was added into the autoclave and stirred for 15 min. The temperature of the autoclave was raised to 180°C, and it was maintained at that temperature for 48 h before being cooled down to room temperature. The products were filtrated, rinsed in deionized water several times, and dried at 80°C overnight.
X-ray diffraction (XRD) was performed with a Rigaku X-ray diffractometer at room temperature, using a quartz monochromator Cu Kα radiation source (λ = 0.1541 nm) under a voltage of 40 kV and a current of 30 mA. Transmission electron microscopy (TEM) was performed with a FEI/TECNAI G2 microscope. Before characterization, the samples were dispersed ultrasonically in ethanol and dropped onto a Cu grid coated with a carbon membrane. Energy-dispersive X-ray spectroscopy (EDX) was performed on an S-4800 scanning electron microscope. Raman spectra were collected under ambient conditions using a RM 2000 microscope confocal Raman spectrometer equipped with a microscope (Renishaw PLC, England). Electrochemical measurements were carried out using a 2032-type coin cell fabricated in an argon-filled glove box (Mbraun, Germany). The working electrode was fabricated in the ratio of 70:20:10 (w/w) active material/carbon black/polyvinylidene difluoride, while lithium foil served as counter and reference electrode. The electrolyte was 1 M LiPF6 dissolved in 1:1 ethylene carbonate (EC) and dimethyl carbonate (DMC). Constant current charge/discharge cycling was conducted on a LAND battery tester (CT2001A) in the voltage range between 3.0 and 0.01 V. Cyclic voltammetry (CV) was performed on a CHI660C electrochemical workstation at a scan rate of 0.1 mV s−1.
where n is the number of electrons per species reaction, A is the apparent surface area of the electrode, D 0 is the diffusion coefficient of Li+ in the solid state, υ is the scan rate, and Δc 0 is the change in Li concentration in the active material.
Figure 6a shows the charge/discharge curves of the electrode containing the Co-doped WS2 nanorods. In the first cycle, the WS2 electrode delivered a lithium insertion capacity of about 668 mAh g−1 when the discharge/charge current density was 50 mA g−1. The first discharge curve shows the insertion plateaus at 1.0 V and 0.75 V. In the second cycle, a lithium insertion plateau at ~2.2 V was observed, as well as a slope starting from 1.75 V and running down to the cut off voltage of 0.01 V. There is a clear distinction in the charge–discharge profile between 0–2 V (~300 mAh g−1) and 2–3 V (~250 mAh g−1). Thus, this material can be regarded as a possible anode material for Li-ion battery in the 0–2 V range and as a cathode material in Li-metal cell technology.
The cycling behavior over 40 cycles is shown in Fig. 6b. For the raw WS2, the charge capacity obviously decreases with cycling, from 520 mAh g−1 for the first cycle to 287 mAh g−1 at the 40th cycle. (The capacity retention is ~55% after 40 cycles.) For the Co-doped WS2 electrode, an irreversible capacity of 668 mAh g−1 is observed in the first cycle, along with a reversible capacity of 568 mAh g−1, which is reduced to 446 mAh g−1 after 20 cycles and 380 mAh g−1 after 40 cycles. The Co-doped WS2 electrode shows a better cycling stability compared with the WS2 precursor electrode. The first cycle coulombic efficiency of the raw WS2 is 81.5%, and it increases with the cycle number, reaching 98.2% by the 40th cycle. For the Co-doped WS2, the coulombic efficiency of the first cycle is 84.7% and over 98% from the 4th cycle, shown in Fig. 6c. The improved electrochemical performance of the Co-doped WS2 sample may be attributed to the small particle size and its one-dimensional structure. However, the charge/discharge capacities of the Co-doped WS2 electrode are lower than those reported for WS2 nanoflakes  and WS2 nanotubes .
The formation mechanism for the nanorods is similar to the synthesis of transition metal-doped Mo x W1−x S2 nanotubes [17, 18]. First, the WS2 powder is exfoliated into lamellae or monolayers by n-butyllithium to form Li x WS2, with the process introducing a large amount of defects, along with large changes in the coordination patterns of the lamellar disulfide, which enables doping with other ions. Then, the CoCl2 aqueous solution is added into the above mixture, a dispersion of single-layer WS2 is formed by the reaction of Li x WS2 with water. After Co2+ cations enter into the WS2 matrix, the bonding properties of the matrix and the bond angles of S–W–S are changed, especially on the sides of layers, which causes the lamellar structure to curl into bamboo-like nanorods.
The decreased capacity of this transition metal-doped WS2 electrode may be because the intercalation of transition metal ions into the WS2 matrix can decrease the distance between layers, which limits the amount of lithium ions electrochemically inserted into the Co-doped WS2. Based on previous research [19–21], lithium ions intercalate into WS2 nanoclusters and defect sites in WS2 nanorods, but these sites are partly saturated with Co2+, so the amount of intercalation of lithium ions will be decreased, and the capacity could thus also be decreased. It can be deduced that for WS2 samples without transition metal-doping or mesoporous WS2, this exfoliation–restacking method will both enhance the charge/discharge capacity and achieve better WS2 cycling stability. Further work is needed in order to further improve the electrochemical performance of WS2 samples via exfoliation and restacking, as well as other modifications.
Bamboo-like Co-doped WS2 nanorods were synthesized by an exfoliation–intercalation–hydrothermal method. WS2 powder was used as the precursor and was exfoliated by n-butyllithium. Co2+ cations were doped into the WS2 matrix through a hydrothermal process in CoCl2 aqueous solution. This method is expected to be applied to other layered materials to obtain the desired morphologies. The Co-doped WS2 nanorods can reversibly store lithium with a capacity of 568 mAh g−1 over a voltage range of 0.01–3.0 V versus Li/Li+. The Co-doped WS2 electrode shows much better cycling stability compared with the raw WS2 electrode.
This work was supported partially by the State Key Laboratory Breeding Base of Green Chemistry-Synthesis Technology, Zhejiang University of Technology and the Priority Research Centers Program through the National Research Foundation of Korea (NRF) funded by the Ministry of Education, Science and Technology (2009-0094047).
This article is distributed under the terms of the Creative Commons Attribution Noncommercial License which permits any noncommercial use, distribution, and reproduction in any medium, provided the original author(s) and source are credited.
- Homyonfer M, Alperson B, Rosenberg Y, Sapir L, Cohen SR, Hodes G, et al.: J. Am. Chem. Soc.. 1997, 119: 2693. COI number [1:CAS:528:DyaK2sXhvV2qtbk%3D] COI number [1:CAS:528:DyaK2sXhvV2qtbk%3D] 10.1021/ja963585zView ArticleGoogle Scholar
- Rapport L, Bilik Y, Feldman Y, Homyonfer M, Cohen SR, Tenne R: Nature. 1997, 387: 791. Bibcode number [1997Natur.387..791R] Bibcode number [1997Natur.387..791R] 10.1038/42910View ArticleGoogle Scholar
- Mdleni MM, Hyeon T, Suslick KS: J. Am. Chem. Soc.. 1998, 120: 6189. 10.1021/ja9800333View ArticleGoogle Scholar
- Chen J, Kuriyama N, Yuan HT, Takeshita HT, Sakai T: J. Am. Chem. Soc.. 2001, 123: 11813. COI number [1:CAS:528:DC%2BD3MXotVCisrs%3D] COI number [1:CAS:528:DC%2BD3MXotVCisrs%3D] 10.1021/ja017121zView ArticleGoogle Scholar
- Yang HB, Liu SK, Li JX, Li MH, Peng G, Zou GT: Nanotechnology. 2006, 17: 1512. COI number [1:CAS:528:DC%2BD28XktVGkt78%3D]; Bibcode number [2006Nanot..17.1512Y] COI number [1:CAS:528:DC%2BD28XktVGkt78%3D]; Bibcode number [2006Nanot..17.1512Y] 10.1088/0957-4484/17/5/058View ArticleGoogle Scholar
- Hu JJ, Zabinski JS, Sanders JH, Bultman JE, Voevodin AA: J. Phys. Chem. B. 2006, 110: 8914. COI number [1:CAS:528:DC%2BD28XjsFWqt7w%3D] COI number [1:CAS:528:DC%2BD28XjsFWqt7w%3D] 10.1021/jp0611471View ArticleGoogle Scholar
- Zhang LL, Tu JP, Wu HM, Yang YZ: Mater. Sci. Eng. A. 2007, 454–455: 487.View ArticleGoogle Scholar
- Lou XW, Zeng CC: Chem. Mater.. 2002, 14: 4781. COI number [1:CAS:528:DC%2BD38XoslSisrk%3D] COI number [1:CAS:528:DC%2BD38XoslSisrk%3D] 10.1021/cm0206237View ArticleGoogle Scholar
- Vollath D, Szabo DV: Mater. Lett.. 1998, 35: 236. COI number [1:CAS:528:DyaK1cXjvVSru7g%3D] COI number [1:CAS:528:DyaK1cXjvVSru7g%3D] 10.1016/S0167-577X(97)00247-4View ArticleGoogle Scholar
- Mirabal N, Lavayen V, Benavente E, Santa Ana MA, Gonzalez G: Microelectron J.. 2004, 35: 37. COI number [1:CAS:528:DC%2BD3sXpt1WisbY%3D] COI number [1:CAS:528:DC%2BD3sXpt1WisbY%3D] 10.1016/S0026-2692(03)00220-9View ArticleGoogle Scholar
- Vanchura BA, He PG, Antochshuk V, Jaroniec M, Ferryman A, Barbash D: J. Am. Chem. Soc.. 2002, 124: 12090. COI number [1:CAS:528:DC%2BD38XntFSisrg%3D] COI number [1:CAS:528:DC%2BD38XntFSisrg%3D] 10.1021/ja025786aView ArticleGoogle Scholar
- Bloise AC, Donoso JP: J. Phys. Chem. B.. 2002, 106: 11698. COI number [1:CAS:528:DC%2BD38XnvVOjuro%3D] COI number [1:CAS:528:DC%2BD38XnvVOjuro%3D] 10.1021/jp012839mView ArticleGoogle Scholar
- Rouxel J: Mater. Res. Bull.. 1978, 13: 1425. COI number [1:CAS:528:DyaE1MXnvFGrtQ%3D%3D] COI number [1:CAS:528:DyaE1MXnvFGrtQ%3D%3D] 10.1016/0025-5408(78)90135-6View ArticleGoogle Scholar
- Zubavichus YV, Slovokhotov YL, Schilling PJ: Inorg. Chim. Acta. 1998, 280: 211. COI number [1:CAS:528:DyaK1cXmtl2ntb8%3D] COI number [1:CAS:528:DyaK1cXmtl2ntb8%3D] 10.1016/S0020-1693(98)00209-6View ArticleGoogle Scholar
- Li YD, Li XL, He RG, Zhu J, Deng ZX: J. Am. Chem. Soc.. 2002, 124: 1411. COI number [1:CAS:528:DC%2BD38XosV2hsA%3D%3D] COI number [1:CAS:528:DC%2BD38XosV2hsA%3D%3D] 10.1021/ja012055mView ArticleGoogle Scholar
- Golub AS, Shumilova IB, Zubavichus YV, Slovokhotov YuL, Novikov YuN, Marie AM, Danot M: Solid State Ionics. 1999, 122: 137. COI number [1:CAS:528:DyaK1MXjsVahsbs%3D] COI number [1:CAS:528:DyaK1MXjsVahsbs%3D] 10.1016/S0167-2738(99)00064-8View ArticleGoogle Scholar
- Li GH, Xu ZD, Chen WX, Nie QL: Chem. J. Chin. Univ.. 2003, 24: 2155.Google Scholar
- Wang SQ, Li GH, He YP, Yin HY, Xu ZD, Zou BS: Mater. Lett.. 2006, 60: 815. COI number [1:CAS:528:DC%2BD2MXhtlWqt7rM] COI number [1:CAS:528:DC%2BD2MXhtlWqt7rM] 10.1016/j.matlet.2005.10.015View ArticleGoogle Scholar
- Sibernagel BG: Solid State Commun.. 1975, 17: 361. Bibcode number [1975SSCom..17..361S] Bibcode number [1975SSCom..17..361S] 10.1016/0038-1098(75)90312-9View ArticleGoogle Scholar
- Feng CQ, Huang LF, Guo ZP, Liu HK: Electrochem. Commun.. 2007, 9: 119. COI number [1:CAS:528:DC%2BD28Xht12gtL7E] COI number [1:CAS:528:DC%2BD28Xht12gtL7E] 10.1016/j.elecom.2006.08.048View ArticleGoogle Scholar
- Wang GX, Bewlay S, Yao J, Liu HK, Dou SX: Electrochem. Solid State Lett.. 2004,7(10):A321-A323. COI number [1:CAS:528:DC%2BD2cXotVKntLc%3D] COI number [1:CAS:528:DC%2BD2cXotVKntLc%3D] 10.1149/1.1788591View ArticleGoogle Scholar
- Poizot P, Laruelle S, Grugeon S, Dupont L, Tarascon J-M: Nature. 2000, 407: 496. COI number [1:STN:280:DC%2BD3cvnslKhtQ%3D%3D]; Bibcode number [2000Natur.407..496P] COI number [1:STN:280:DC%2BD3cvnslKhtQ%3D%3D]; Bibcode number [2000Natur.407..496P] 10.1038/35035045View ArticleGoogle Scholar
- Virsek M, Jesih A, Milosevic I, Damnjanovic M, Remskar M: Surf. Sci.. 2007, 601: 2868. COI number [1:CAS:528:DC%2BD2sXmvVeht74%3D]; Bibcode number [2007SurSc.601.2868V] COI number [1:CAS:528:DC%2BD2sXmvVeht74%3D]; Bibcode number [2007SurSc.601.2868V] 10.1016/j.susc.2006.12.050View ArticleGoogle Scholar
- Wang Q, Li JH: J. Phys. Chem. C.. 2007, 111: 1675. COI number [1:CAS:528:DC%2BD2sXovVWq] COI number [1:CAS:528:DC%2BD2sXovVWq] 10.1021/jp066655pView ArticleGoogle Scholar
- Levi MD, Aurbach D: J. Electroanal. Chem.. 1997, 421: 79. COI number [1:CAS:528:DyaK2sXivV2lsLw%3D] COI number [1:CAS:528:DyaK2sXivV2lsLw%3D] 10.1016/S0022-0728(96)04832-2View ArticleGoogle Scholar